Tải bản đầy đủ - 0trang
2?Pretreatment of Native Biomass
4 Application of Ionic Liquids
Fig. 4.1 Generalized chemical structure of lignin and schematic for its conversion into
monomeric aromatic products. Reactions which cleave aryl–ethers and aryl–alkyl linkages would
enable conversion of lignin into valuable aromatic chemicals. Reprinted from , copyright
(2011), with permission from Elsevier
cellulose or glucose oligomers can fail to translate to native biomass. In lignin,
each type of linkages in the constituting monolignols provides a possible pathway
for biomass delignification (Fig. 4.1) [25–28]. Developing a unique IL pretreatment that would be suitable for multiple feedstocks represents a tremendous
4.2.2 Dissolution of Biomass in Ionic Liquids
A wide variety of biomass feedstock/IL combinations has been studied for their
potential in biomass pretreatment. Multiple wood species have been studied:
poplar , spruce [7, 30–34], eucalyptus [31, 32], pine [4, 6, 7, 31, 32, 35–37],
maple [25, 38], Metasequoia glyptostroboides , red oak , common beech
, cork , and Japanese fir . Other biomass feedstocks currently under
investigation include grasses, such as switchgrass [41, 42], Miscanthus grasses [26,
43], and agricultural wastes, such as corn stovers [6, 33, 35, 43–45], wheat straw
 and rice straw [6, 35, 46].
Among the most successful and widely used ILs in native wood pretreatment
are the imidazolium-based ILs with the chloride or acetate anion. The ILs 1-allyl3-methylimidazolium chloride ([AMIM][Cl]) and [BMIM][Cl] could dissolve
M. Lucas et al.
maple wood flour at solubilities above 30 g/IL kg at 80°C under nitrogen atmosphere after 24 h . Ball-milled pine powder and spruce sawdust (size
0.1–2 mm) were completely dissolved in [BMIM][Cl] and [AMIM][Cl] at a
weight ratio of up to 8% at 80–110°C in 8 h with mechanical stirring .
[AMIM][Cl] was able to dissolve completely 5 wt% of spruce, silver fir, beech,
chestnut wood chips (particle size 1–2 mm) at 90°C in 12 h, whereas the same
wood samples were only partially dissolved in 1-ethyl-3-methylimidazolium
chloride ([EMIM][Cl]), [BMIM][Cl], and 1,3-dimethylimidazolium dimethylphosphate ([MMIM][Me2PO4]) in the same conditions . The IL 1-ethyl-3methylimidazolium chloride ([EMIM][Cl]) can partially dissolve wheat straw
and pine wood particles (\1 mm, 5 wt%) at 100°C in 24 h, [BMIM][Cl] can
only partially dissolve wheat straw, and 1-ethyl-3-methylimidazolium acetate
([EMIM][OAc]) could dissolve neither . Ground pine, poplar, eucalyptus, and
oak were dissolved in [BMIM][Cl] with a 5 wt% solubility at 100°C. After 24 h,
about 45 wt% of the cellulosic material was extracted from the native biomass.
The extraction rates were higher for softwoods, such as pine and poplar.
C Nuclear Magnetic Resonance (NMR) confirmed the presence of dissolved
polysaccharides in the wood/IL mixture .
[EMIM][OAc] dissolved spruce, beech, chestnut completely (5 wt%), but not
silver fir . In another study, [EMIM][OAc] could dissolve 5 wt% of red oak
(particle size 0.125–0.250 mm) completely in 25 h at 110°C, while it took 46 h
to dissolve 5 wt% of southern yellow pine in the same conditions .
Pretreatment of maple wood flour with [EMIM][OAc] or 1-butyl-3-methylimidazolium acetate ([BMIM][OAc]) at 90°C increased significantly the sugar yield
and the amount of extracted lignin . Pretreatment with 1-butyl-3-methylimidazolium methyl sulfate ([BMIM][MeSO4]) at the same temperature for the
same duration resulted in sugar yields comparable to the untreated wood
flour and an amount of extracted lignin lower than with [EMIM][OAc] or
[BMIM][OAc]. This was explained by the fact that [BMIM][MeSO4] only
delignified the middle lamella and not the primary cell wall and cellulose-rich
secondary cell wall. Also, the [EMIM][OAc] or [BMIM][OAc] pretreatment for
12 h reduced the wood fiber diameter from an average of 250 lm in the
untreated flour to about 17 lm. Pretreatment with [BMIM][MeSO4] had no effect
on the wood fiber diameter .
Other combinations of IL/native wood were studied. Dry wood (Metasequoia
glyptostroboides, 60 mesh sawdust) was partially dissolved in 1-butyl-3-allylimidazolium chloride ([BAIM][Cl]) or 1-methyl-3-allylimidazolium chloride
([MAIM][Cl]) at a weight ratio from 4.5:1 to 10.5:1 (60–90°C for 10–40 min)
. Phenyl-containing ionic liquids were synthesized to see if the aromatic
p-systems would be better at disrupting the strong p–p interactions between aromatic groups in lignin. Indeed, after the wood was dissolved in 1-benzyl-3methylimidazolium chloride ([BzMIM][Cl]), the solution was clear, free of any
residual lignin . Ball-milled poplar was soluble in 1-allylpyridinium chloride,
cyanomethylpyridinium chloride, and pyridinium chloride within 1 h at 60°C with
solubilities ranging from 35 to 80 mg/g .
4 Application of Ionic Liquids
In addition to woods, ILs could at least partially dissolve or delignify other
feedstocks, including leaves and agricultural wastes. Triticale straw, flax shives,
and wheat straw were soluble in [EMIM][OAc] and [BMIM][Cl] . The dissolution of shredded oil palm fronds in [BMIM][Cl] was studied for temperatures
ranging from 60 to 100°C . Lignin was extracted from bagasse using the
IL 1-ethyl-3-methylimidazolium alkylbenzenesulfonate at high temperatures
(170–190°C) . Rice straw powder (\2 mm) could be dissolved in [BMIM]
[Cl], [EMIM][Cl], and [EMIM][OAc] completely in 24 h at 130°C. The amount of
regenerated cellulose and glucose after enzymatic hydrolysis was highest for
[EMIM][OAc] . Milled corn cob had solubilities above 30 g/kg at 130°C in
1-methyl-3-methylimidazolium dimethylphosphite ([MMIM][DMP]), 1-ethyl-3methylimidazolium diethylphosphate ([EMIM][DEP]), 2-ethyl-3-methylimidazolium dimethylphosphite ([EMIM][DEP]), [BMIM][Cl], and 1-butyl-1-methylpyrrolidinium chloride ([BMPy][Cl]). Pretreatment with chloride ILs resulted in
the doubling of reducing sugar yield after enzymatic hydrolysis .
4.2.3 Effect of Ionic Liquid Chemical Composition
The nature of the anion played a major role in the dissolution of biomass. For
example, [EMIM][OAc] was more effective than [EMIM][Cl] in the dissolution of
southern yellow pine . The chloride anion combined with the [BMIM] cation
was effective in the dissolution of maple wood flour. Substitution of the chloride
anion with the tetrafluoroborate or hexafluorophosphate anions made the maple
wood flour insoluble . Maple wood flour pretreated in [EMIM][OAc] and
[BMIM][OAc] at 90°C for 6 h resulted in a decrease in cellulose crystallinity,
higher glucose, and xylose yields. In contrast, pretreatment with [BMIM][MeSO4]
had little effect on the biomass cell structure, sugar yields, and cellulose crystallinity, compared to untreated wood flour .
The ability to dissolve biomass was related to the anion basicity. [EMIM][OAc]
was a better solvent than [BMIM][Cl] for southern yellow pine and red oak (particle
size 0.125–0.250 mm), due to the increased basicity of the acetate anion and also its
lower viscosity and melting point . Cork powder remained insoluble in
[EMIM][Cl] and [BMIM][Cl] after 4 h at 100°C. Replacing the chloride anion with
a lactate or ethanoate anion improved the cork dissolution significantly. ILs based
on the cholinium cation and alkanoate anions were more effective in the cork
dissolution. Among the alkanoate anions included in the study, the increasing alkyl
chain length (ethanoate, butanoate, hexanoate) led to an increase in biomass dissolution efficiency, attributed to an increase in the basicity of the anion .
The structure of the cation plays a role in the melting point of the IL. Alkyl
groups on the imidazole tend to lower the melting temperature, and enhance wood
liquefaction and processability of the wood solution. For example, wood dissolution was more effective in 1-butyl-3-allylimidazolium chloride ([BAIM][Cl]),
then in 1-methyl-3-allylimidazolium chloride ([MAIM][Cl]) .
M. Lucas et al.
4.2.4 Effect of Temperature
Most IL pretreatments were conducted at high temperatures ranging from 70
to 190°C [7, 22, 25, 27, 36, 37, 43, 48–50]. Higher sugar yields are usually
reported for pretreatments at higher temperatures for longer times [7, 22, 25, 27,
50]. Wood dissolution at temperatures above 100°C was faster in [BMIM][Cl]
and [AMIM][Cl] . Short pretreatments at higher temperatures resulted in
higher glucose yields from oil palm fronds . Increasing temperatures from 50
to 130°C during the dissolution of maple wood flour in [EMIM][OAc] increased
the amount of extracted lignin and reduced the recovered wood flour . In
another study, increasing the temperatures from 70 to 150°C increased the solubility of lignin in triticale straw residues. The cellulose and hemicellulose
content in the residues decreased with higher temperatures. The IL treatment at
higher temperatures also resulted in higher glucose yields after enzymatic
hydrolysis. More than 95% of the initial cellulose extracted above 130°C after
11 h was hydrolyzed . This can be partially explained by the fact that, at
higher temperatures, the self-diffusion coefficients of the IL anions and cations
increase dramatically .
Another possible explanation of the benefits of high temperatures on biomass
pretreatment is the improved access of enzymes to cellulose. The surface area,
pore size distribution, and pore volume of switchgrass (3 wt%, 40 mesh) pretreated
with [EMIM][OAc] at 110–160°C for 3 h, were measured by nitrogen porosimetry. The switchgrass pretreated at 160°C adsorbed significantly more gas than
the untreated sample or the one treated at 120°C, with a specific surface area 30
times higher (15.8 m2/g at 160°C, 0.7 m2/g at 120°C, and 0.5 m2/g for the
untreated sample). The increased surface area and pore volume were correlated
with an increase in the initial rates of enzymatic hydrolysis. After 30 min of
hydrolysis with cellulases from Trichoderma reesei, the concentration of reducing
sugars in the broth was 2.84 g/L for a 3-h IL treatment at 110°C and 7.44 g/l for
the sample treated at 160°C. The lignin removal efficiency also increased from
25% at 110°C to 74% at 160°C. The improved delignification and sugar yields
observed for pretreatments above 150°C was attributed mostly to the softening or
melting of lignin. The average glass transition temperature of lignin is around
165°C, but varies considerably depending on its chemical composition and the
ratio of monolignol units .
Cellulose degradation was reported when IL pretreatment is conducted at
higher incubation time and higher temperature, leading to lower sugar yields after
enzymatic hydrolysis . There was evidence of degradation of the IL and cellulose, when pine wood chips were pretreated in [EMIM][OAc] at 110°C for 16 h.
The appearance of additional peaks on 13C NMR spectra of the pine/IL solution
was attributed to the generation of glucose oligomers and the degradation of
4 Application of Ionic Liquids
4.2.5 Effect of Density
[AMIM][Cl] dissolved Eucalyptus grandis, southern pine sawdust (particle size
0.1–2 mm) and Norway spruce thermomechanical pulp almost completely in 5 h at
120°C. IL pretreatment of southern pine improved the glucose yield after enzymatic
hydrolysis from 7 to 17 wt%. But the improvement of the glucose yield after IL
pretreatment was found to decrease with increasing wood density. Higher density
wood (Eucalyptus grandis) requires an IL pretreatment at a higher temperature than
low-density wood (southern pine) to achieve the same pretreatment efficiency .
Hardwoods such as red oak usually have a higher density than softwoods such as
pine, but softwoods also tend to have higher lignin content. Lignin in softwoods is
also rich in guaiacyl units, while lignin in hardwoods is a mixture of guaiacyl and
syringyl units . Similarly, wheat straw (low lignin content) could be dissolved in
[EMIM][OAc] with acetic acid at a lower temperature (100°C) than pine wood
(higher lignin content) (120°C) for the same particle size (\1 mm) .
Generally, the high viscosity of the IL affects negatively the overall efficiency of
the pretreatment . The IL viscosity depends on the IL chemical composition and
temperature. For example, [AMIM][Cl] has a lower viscosity than [BMIM][Cl],
which enabled wood dissolution at a lower temperature (80°C instead of 110°C).
Dissolution in ILs with aromatic substituents, such as [BzMIM][Cl] and 1-methyl3-m-methoxylbenzylimidazolium chloride, required higher temperatures (130°C)
to achieve the same wood solubility, which was attributed to their higher melting
temperatures and viscosities . However, the viscosity of the wood/IL mixture
also increases with the wood dissolution over time with the accumulation of
extracted products and generation of by-products . The viscosity of cellulose
solutions in [EMIM][OAc] or [BMIM][Cl] was found to increase with the cellulose concentration [51, 52].
One way to decrease the viscosity of the wood/IL mixture is to increase the
temperature, but this solution is energy-intensive and can accelerate the degradation of the IL . Another method consists in the addition of a co-solvent with
lower viscosity. The viscosity of a wood/[BMIM][Cl] mixture was reduced by the
addition of deuterated dimethyl sulfoxide, which had no noticeable effect on the
wood dissolution efficiency . In another study, [BzMIM][Cl] was blended with
[AMIM][Cl] to reduce its viscosity without significant efficiency loss. Biomass
dissolution could occur at a lower temperature and even at room temperature in the
less viscous [AMIM][Cl] .
During wood dissolution in [BAIM][Cl] and [MAIM][Cl] with AlCl3 as a catalyst,
increased acidity led to a decrease in viscosity, which was attributed to the formation
of AlCl4 and Al2Cl7 that weakens the hydrogen bonds in ionic liquids .
M. Lucas et al.
4.2.7 Acid Hydrolysis
Several acids served as catalysts with [BMIM][Cl] for the hydrolysis of corn stalk:
hydrochloric acid, sulfuric acid, nitric acid, phosphoric acid, and maleic acid.
Overall, hydrochloric acid was the most efficient catalyst. Sulfuric and nitric acids
were also efficient, but required a higher loading to achieve the same yield in
reducing sugars. At the same temperature (100°C), reactions with phosphoric and
maleic acids were much slower than with the other acids, even at high loadings.
The combination of hydrochloric acid (7 wt%) and [BMIM][Cl] was efficient in
the hydrolysis of corn stalk, rice straw, pine wood, and bagasse . Faster
degradation of cellulose and hemicellulose was also observed at higher temperatures and for longer pretreatment times for Eucalyptus grandis . The
weight loss increased with the amount of hemicellulose, which was higher in
softwoods (spruce and pine). More carbohydrates (polysaccharides and lignin)
were hydrolyzed as the acid concentration increased . Trifluoroacetic acid
(0.2 wt%) also served as an acid catalyst in the dissolution of loblolly pine in
[BMIM][Cl] at 120°C. Its effect was similar to sulfuric acid H2SO4 at the same
molar concentration. After a 2-h treatment, 62 wt% of the loblolly pine was
converted to soluble products. No further increase in the yield was seen after a
4-h treatment . The addition of AlCl3 led to a decrease in pH in a mixture of
wood (Metasequoia glyptostroboides) and [BAIM][Cl] and [MAIM][Cl], which
accelerated the dissolution of wood at a lower temperature. The amount of
insoluble residues in the IL and pH decreased with increasing AlCl3 amount. The
selection of the metal chloride affected the pH and the liquefaction efficiency:
AlCl3 led to lower pH than SnCl2 and FeCl3. The stronger acidity led to higher
liquefaction efficiency . These results were consistent with a previous study
in which the initial acid hydrolysis rates of cellobiose increased with increasing
acid strength. The conversion of cellobiose to glucose was much faster for acids
with negative pKa values, such as methanesulfonic acid (pKa = -1.9) and
sulfuric acid (pKa = -3) .
From these results, it was argued that biomass does not dissolve in ILs
directly, but that it needs to be hydrolyzed first before the dissolution of the
hydrolysis products. Pine wood and wheat straw (mesh size smaller than 1 mm)
were dissolved in [EMIM][OAc] with acetic acid as catalyst. After dissolution,
a drop in pH was observed with formation and accumulation of acetic acid in
the IL/biomass solution. The addition of acetic acid to [EMIM][OAc] accelerated the dissolution of wheat straw. After dissolution and addition of water,
the precipitate contained an amount of lignin that increased with the amount of
acetic acid added, suggesting that acetic acid also acted as a co-solvent for
Indeed, IL pretreatments with acid may increase the yield of reducing sugars
following enzymatic hydrolysis, but they also promote the degradation of cellulose
and hemicellulose when conducted at higher temperatures and for longer times
[6, 32, 47, 53]. Faster degradation of cellulose and hemicellulose was observed at
4 Application of Ionic Liquids
higher temperatures and for longer pretreatment times for Eucalyptus grandis .
For the acid hydrolysis of loblolly pine in [BMIM][Cl], the yield of monosaccharides reached a maximum after 2 and 0.5 h of pretreatment at 120 and 150°C,
respectively . Similarly, the yield of reducing sugars after hydrolysis of corn
stalk in [BMIM][Cl] with HCl reached a maximum for an incubation time of
30 min at 100°C . High performance liquid chromatography (HPLC) of residues from the acid-catalyzed pretreatment of loblolly pine in [BMIM][Cl] showed
that the monosaccharides from biomass reacted by dehydration to form other
compounds, such as 5-hydroxymethylfurfural and furfural . 31P NMR spectra
of the recycled IL after pretreatment of Eucalyptus grandis exhibited signatures
from 5-hydroxymethylfurfural, acetol, 2-methoxy-4-methylphenol, catechol, and
acetic acid . Fourier-transform infrared (FTIR) spectroscopy of corn stalk after
pretreatment in [BMIM][Cl] with sulfuric acid showed the functionalization of
lignin with sulfonic groups . The generation of these by-products reduces the
total reducing sugar yield, can affect the enzymatic hydrolysis of the remaining
cellulose and complicate the recycling of the IL.
In addition to acids, other catalysts such as Li salts (LiCl, LiBr, LiAc, LiNO3,
or LiClO4) were added to enhance the dissolution of cellulose in [EMIM][OAc].
It was believed that the lithium cation can disrupt the hydrogen bonding network
in cellulose .
Two polyoxometalates, an acidic form H5[PV2Mo10O40] and an [EMIM][OAc]
compatible form [1-ethyl-3-methylimidazolium]4H[PV2Mo10O40], were prepared
and used as catalysts for the dissolution of southern yellow pine (particle size
\0.125 mm, 5 wt%) in [EMIM][OAc] at 110°C . The addition of 0.5 wt%
acidic polyoxometalate reduced the time for complete dissolution of pine from 46
to 15 h. The regenerated cellulose contained significantly less lignin, with limited
losses in cellulose. The [EMIM]-compatible form improved delignification, but
with greater cellulose losses in the regenerated cellulose .
4.2.9 Pretreatment with Ammonia
An ammonia pretreatment prior to IL dissolution improved delignification of
biomass and enhanced recyclability. The rice straw (particle size 2–5 mm) was
first treated with ammonia (10%) at 100°C for 6 h. After filtering and drying steps,
it was dissolved in [EMIM][OAc] at 130°C for 24 h. The ammonia pretreatment
step reduced the time for complete dissolution in IL from 24 to 6 h. It increased
slightly the amount of regenerated cellulose after the IL treatment for \24 h. The
major improvement was the significant increase in the glucose conversion rate of
M. Lucas et al.
97% (compared to the amount of regenerated cellulose) with the ammonia
pretreatment, compared to the 78% rate without ammonia pretreatment. This
improvement allowed for a significant reduction in the amount of cellulases
necessary for cellulose hydrolysis: despite a reduction of the cellulase concentration by a factor 10, the cellulose conversion rate remained at 83% .
4.2.10 Microwave Heating and Ultrasounds
The complete dissolution of native biomass in ILs using conventional heating (oil
bath) may take several hours at high temperatures. In order to reduce the energy
costs associated with heating, a commercial microwave oven was used to heat the
wood/IL mixture before it was heated using a conventional oil bath. The application of 100 pulses of 3 s reduced the time necessary to dissolve pine sawdust
(particle size 0.125–0.250 mm) completely from 46 to 16 h . Microwave
irradiation also accelerated the production of 5-hydroxymethylfurfural and furfural
directly from milled corn stalks, rice straws, and pine wood, reducing the reaction
time down to a few minutes .
Ultrasounds can also accelerate the complete dissolution of cellulose in
[BMIM][Cl] and [AMIM][Cl] from several hours to several minutes . The
exposure of pine sawdust (particle size 0.125–0.250 mm) to 1 h of ultrasound at
40°C before IL treatment reduced the time necessary to dissolve the sample from
46 to 23 h .
4.2.11 Biomass Size Reduction
The dissolution of Norway spruce in [BMIM][Cl] or [AMIM][Cl] depended on the
size of the biomass. Whereas ball-milled powder and spruce sawdust (size
0.1–2 mm) were completely dissolved at 80°C in several hours, it took several
weeks to dissolve wood chips (5 9 5 9 1 mm3) at 130°C in the same ILs.
In general, dissolution was fastest for ball-milled wood, followed by sawdust
(particle size 0.1–2 mm), thermomechanical pulp fibers, and wood chips .
A similar size effect was observed for southern pine and red oak wood chips , and
rice straw . Ball-milling of Norway spruce TMP and southern pine increased the
glucose yield after IL pretreatment and enzymatic hydrolysis, by opening access to
the wood structure for enzymes. The same effect, which became more significant
with milling time, was also observed for corn stovers. The molecular weight of ballmilled corn stovers decreased with increasing milling time .
The size reduction effect could be explained by the increase of effective surface
area and the improved access of enzymes to the biomass cellulose. However,
feedstock size reduction through mechanical grinding is energy-intensive .
Also, ball-milling for several days can lead to significant degradation and chemical
4 Application of Ionic Liquids
modification of cellulose and lignin, as well as the generation of soluble species
that reduces the recyclability of the IL [31, 33, 57]. It was reported that extensive
ball-milling causes cleavage of aryl–ether linkages in lignin and the generation of
phenolic hydroxyl groups .
4.2.12 Comparison with Other Pretreatments
Few studies have directly compared the efficiency of IL pretreatments to other
pretreatments, such as the ammonia or organosolv pretreatment. Rice straw
particles were pretreated with [EMIM][OAc] (1 g biomass in 20 ml of [EMIM][OAc] at 130°C for 24 h) or ammonia (1 g biomass in 10 ml of 10 vol.%
ammonia at 100°C for 6 h). In these conditions, the amount of cellulose regenerated was comparable for the two pretreatments. However, the conversion rate of
cellulose to glucose was significantly higher with the IL pretreatment and the
improvement due to IL was most remarkable for larger particles ([10 mm) .
In another study, switchgrass was subjected to an acid pretreatment (3 wt%
biomass in 1.2% sulfuric acid heated at 160°C for 20 min) or an IL pretreatment
with [EMIM][OAc] (3 wt% biomass heated at 160°C for 3 h). Analysis of the
recovered biomass after IL pretreatment showed lower lignin content and higher
hemicellulose content, compared to the recovered biomass after acid pretreatment.
X-ray diffraction measurement of the cellulose crystallinity showed a significant
decrease in crystallinity after IL pretreatment, whereas the acid pretreatment
caused an increase in crystallinity, which was attributed to the preferential
breakdown of the amorphous cellulose during the acid pretreatment. Scanning
electron microscopy showed that the cell wall structure was mostly preserved
during the acid pretreatment, while the IL pretreatment left no fibrous structure.
For the same enzyme loading, the enzymatic hydrolysis had faster kinetics and
higher reducing sugar yields after the IL pretreatment. After a 24 h saccharification process, 96% of the cellulose was hydrolyzed for the IL-pretreated sample,
while only 48% were hydrolyzed for the acid-pretreated sample .
4.2.13 Water Adsorption as an Issue
The wide range of biomass solubility in ILs reported in the literature could be
partially explained by the contamination with water, which can significantly
affect their physicochemical properties . Even hydrophobic ILs, such as
1-ethyl-3-methylimidazolium bis(trifluoromethylsulfonyl)imide ([EMIM][Tf2N]),
are hygroscopic and can contain up to 25% of water (molar ratio) when exposed to
an environment with a relative humidity of 81% . Water can also be produced
during the reaction of biomass with IL by the hydrolysis of acetate groups .
Traces of water can be detected by 1H NMR or IR spectroscopy . They can be
M. Lucas et al.
quantified by Karl-Fischer titration or gravimetrically . Water can be removed
in a vacuum oven or in a freeze dryer [7, 61]. Its presence complicates the
IL recycling and removal is energy-intensive.
Addition of water above 4 wt% to loblolly pine wood before its pretreatment in
[BMIM][Cl] led to a notable decrease in soluble products, monosaccharides, and
5-hydroxymethylfurfural. This was attributed to the competition with the cellulose
hydroxyl groups to form hydrogen bonds with Cl- ions . The presence of
water reduced the solubility of wood in ILs and the yield of sugars released in the
dissolution of maple wood flour in [BMIM][OAc] and [EMIM][OAc] . Water
also prevented the IL from effectively reducing the cellulose crystallinity .
Water can also prevent the formation of by-products such as 5-hydroxymethylfurfural during the dissolution of cellulose in [EMIM][Cl] catalyzed by HCl or
The IL hygroscopicity is the result of the adsorption of water on the IL surface,
diffusion from the surface and/or the formation of complexes through hydrogen
bonding [59, 63, 64]. The hygroscopicity depends on the IL composition and
structure . Adsorption would depend on the charge distribution and structure of
the cation and anion, while diffusion would be affected by the IL viscosity .
The length of alkyl chains and substitution on the cation ring (e.g., pyridinium,
imidazolium) affected the mutual solubility of the IL with water [65, 66]. For ILs
with the [EMIM] cation, water uptake increased with different anions in the following order: dicyanamide \ diethyl phosphate \ chloride \ acetate .
4.2.14 Presence of Impurities
As-produced commercial ILs can contain halides, water, organics, and unreacted
salts from their synthesis . The presence of impurities could explain differences in performance between identical ILs from different manufacturers . The
presence of residual chloride salts can dramatically increase the viscosity of the IL
and decrease its density. 1H NMR studies suggested that the viscosity increase may
be due to the increase in hydrogen bonding between the chloride anion and the
protons of the imidazolium cation . Halides in a few ILs, such as 1-butyl3-methylimidazolium tetrafluoroborate ([BMIM][BF4]), can be removed by water
washing, but the water excess would have to be removed under vacuum or by
Impurities, such as methyl imidazole (source of imidazolium-based ILs), can
affect the pH of the solution and reduce ion concentrations . The mixture of
water with commercially available [EMIM][Cl] (equal weight) has a pH around 7,
whereas the mixture of purified [EMIM][Cl] and water (equal weight) has a pH of
5.12. The addition of methyl imidazole to the purified IL brought the pH back
to around 7. The lower pH obtained with the purified was attributed to the
enhanced water dissociation and the resulting higher ion concentrations. Ab initio
simulations predicted enhanced water dissociation at a high ionic strength (high
4 Application of Ionic Liquids
IL content) or at a high dielectric constant (high water content). The ions from the
enhanced water dissociation in purified ILs could effectively catalyze the conversion of cellulose to sugars without the addition of acid catalysts .
4.3 Mechanism of Delignification and Cellulose Dissolution
4.3.1 Analytical Techniques
Advances in a variety of analytical techniques have provided valuable insight into
the mechanisms involved in delignification and cellulose dissolution. Optical and
fluorescence microscopy enabled the study of wood expansion (Fig. 4.2) [70, 71]
and switchgrass dissolution  in ionic liquids at the micron scale. Distinct
autofluorescence from cellulose and lignin signatures distinguish the cellulose-rich
cell walls and the lignin-rich cell corners and middle lamellae in poplar and
switchgrass [42, 70, 71]. Optical and scanning electron microscopies have been
particularly useful in visualizing IL interacting with heterogeneous native biomass.
They revealed structural changes after dissolution, regeneration, and chemical
functionalization [22, 30, 36, 38, 41, 42, 44, 72].
X-ray diffraction provided an insight into structural changes occurring at the
atomic scale in cellulose during its dissolution and regeneration [7, 36, 38, 71, 73].
It was used to monitor in situ the loss of cellulose crystallinity in poplar, ramie
fibers , switchgrass, eucalyptus, and pine wood . After the regeneration of
dissolved pine and spruce sawdust, X-ray diffraction revealed a change of crystal
structure from the native cellulose I to the cellulose II structure [7, 36]. Neutron
scattering was used to estimate the surface roughness of switchgrass, eucalyptus,
and pine after their IL pretreatment .
These structural changes were supplemented by analyses of the biomass
chemical composition. The distinct Raman signatures of cellulose and lignin have
made hyperspectral Raman imaging a powerful tool to map the chemical composition of native biomass  and its evolution during pretreatments [70, 71].
IR spectroscopy was commonly used to assess purity [4, 39, 42], loss of hemicelluloses/lignin after the dissolution [36, 42], chemical functionalization [6, 7, 30, 48],
cleavage of b–O–4 bonds in lignin models [75, 76]. It can also probe the interactions
between the anion and cation in the IL and the hydrogen bonding network . FTIR
spectroscopy combined with principal component analysis was used to distinguish
lignins from bagasse, softwoods, and hardwoods . Efforts were made to use
IR spectroscopy as a method to quantify glucose and cellobiose in [EMIM][OAc].
The IR absorption of multiple bands in glucose and cellobiose was found to vary
with concentration and empirical nonlinear relations between the absorbance and the
concentration were derived .
Optical absorption spectroscopy offers a quick way to quantify the
saccharification of purified substrates, such as Avicel, and native biomass.